Research Article  Open Access
Mosaic Structure Characterization of the AlInN Layer Grown on Sapphire Substrate
Abstract
The 150 nm thick, (0001) orientated wurtzitephase Al_{1−x}In_{x}N epitaxial layers were grown by metal organic chemical vapor deposition on GaN (2.3 µm) template/(0001) sapphire substrate. The indium (x) concentration of the Al_{1−x}In_{x}N epitaxial layers was changed as 0.04, 0.18, 0.20, 0.47, and 0.48. The Indium content (x), lattice parameters, and strain values in the AlInN layers were calculated from the reciprocal lattice mapping around symmetric (0002) and asymmetric (10–15) reflection of the AlInN and GaN layers. The mosaic structure characteristics of the AlInN layers, such as lateral and vertical coherence lengths, tilt and twist angle, heterogeneous strain, and dislocation densities (edge and screw type dislocations) of the AlInN epilayers, were investigated by using highresolution Xray diffraction measurements and with a combination of WilliamsonHall plot and the fitting of twist angles.
1. Introduction
Because of the large band gap, large breakdown field, and strong spontaneous and piezoelectric polarization field’s properties of the IIInitride materials systems, they have been used in optoelectronic devices, such as light emitting diodes, blue/ultraviolet lasers, metalsemiconductor field effect transistors, modulationdoped field effect transistors, photodetectors, and high temperature/high power electronic devices [1–3]. The structural quality of GaN based alloys can significantly affect its electrical and optical properties and also the performance of devices [1–7]. One of the most common problems for the growth of group GaN based alloys heterostructures is the lattice constant mismatch between the binary and ternary compounds of Ga, In, Al, and N elements [1–4, 7–9]. The mismatches in multilayered structures result in strain and potentially crack formation that deteriorates the performance of devices [7, 10, 11]. Many studies have been performed to improve the structural quality of GaN based alloys and the performance of devices, such as increasing the Al composition of an AlGaN barrier, using a thin AlN spacer layer at the AlGaN/GaN interface, and replacing the GaN by InGaN as the channel and AlGaN by AlInN layer as a barrier [12, 13]. Among these studies, it is possible to grow a latticematched AlInN layer on GaN layer for an In concentration of ~18% [12–14]. Due to its promising electronic properties, polarization effects, and high thermal stability, the latticematched AlInN material system has become of interest for electronic applications [15–17]. The latticematched AlInN barrier in the AlInN/GaN high electron mobility transistor (HEMTs) shows superior performance compared to the AlGaN/GaN HEMTs [12, 13]. In addition, the use of appropriate AlInN enables the fabrication of latticematched GaNbased heterostructures that can be used for highperformance laser diodes [17]. Furthermore, AlInN alloys can possibly be used for light emitters and detectors operating in extremely wide spectral regions covering from deep infrared to UV since the alloys bandgap energy can range from 0.7 eV (InN) to 6.2 eV (AlN) [1–3].
Despite the many advantages for devices, the growth of AlInN alloys over the full compositional range is extremely difficult due to the large differences in the chemical and physical parameters between AlN and InN. Due to the different growth conditions of AlN and InN and the expected large immiscibility gap of the ternary alloy, the growth of AlInN in the whole compositional range is challenging [18–20].
The GaN based structures are usually grown on highly latticemismatched substrates, such as sapphire, SiC, or Si [4, 11]. The large lattice mismatch and large difference in the thermal expansion coefficients between the GaN layer and the substrates (sapphire, SiC, and Si) cause a high level of inplane stress and threading dislocation generation in the epitaxial layers and reduce the crystal quality of the GaN layers during the growth [4, 5, 8–11]. The high level of inplane stress and threading dislocation in the epitaxial layers affect the performance reliability of the device [1–5, 10]. The distorted GaN based semiconductor material can be described with mosaic structures that can be characterized by means of vertical and lateral coherence lengths (average size of the mosaic blocks) twist and tilt angle, heterogeneous strain, and dislocation densities (edge and screw type threading dislocations) [8, 9, 21–31]. The tilt describes the rotation of the mosaic blocks out of the growth plane and the twist in their inplane rotation. The average absolute values of the tilt and twist are directly related with the full width at half maximum (FWHM) of the corresponding distributions of the crystallographic orientations [21, 23–31].
In this study, we present investigations of the mosaic properties of grown in the composition range 0.04, 0.18, 0.20, 0.47, and 0.48 on GaN/sapphire structures by metal organic chemical vapor phase deposition (MOCVD). The main aim of the work is to grow AlInN layers on a GaN template with a wide range of indium content and investigate the mosaic structure parameters of the AlInN layers. The mosaic structure features (such as lateral and vertical coherence lengths, tilt and twist angle, and heterogeneous strain) and dislocation densities (edge and screw type dislocations) of hexagonal AlInN layers were determined by HRXRD measurements. Additionally, atomic force microscopy (AFM) imaging was performed in order to obtain detailed knowledge on the surface morphology of the samples.
2. Experimental Procedure
Epitaxial (, 0.18, 0.20, 0.47, and 0.48) layers were grown on doublepolished 2inch diameter sapphire substrates in a low pressure MOCVD reactor (Aixtron 200/4 HTS) by using trimethylgallium (TMGa), trimethylaluminum (TMAl), trimethylindium (TMIn), and ammonia as Ga, Al, In, and N precursors, respectively. Before the epitaxial growth, the Al_{2}O_{3} substrate was annealed at 1110°C for 15 min in order to remove surface contamination. The buffer structures of all the samples consisted of a 15 nm thick, lowtemperature (710°C) GaN nucleation layer, and high temperature (1100°C) 2.3 μm GaN template layer. After GaN template layer growth, a nominally 150 nm undoped AlInN layer was grown. In this study, five different samples were grown, with a different indium concentration, on GaN template layers (Figure 1). The In content was changed by changing the growth temperature and TMIn/(TEGa+TMIn) ratio. The growth temperatures and the TMIn/(TEGa+TMIn) ratio of the samples are 900, 830, 830, 730, and 745°C and 0.69, 0.69, 0.43, 0.75, and 0.75 for an indium content of 0.04, 0.18, 0.20, 0.47, and 0.48, respectively. The samples were identified with consideration of the indium content as samples A, B, C, D, and E, 0.04, 0.18, 0.20, 0.47, and 0.48, respectively.
The crystalline quality of the GaN layers was examined by high resolution Xray diffraction (HRXRD). The Xray diffraction was performed using a Rigaku SmartLab highresolution diffractometer system, delivering CuKα1 (1.544 Å) radiation, and 4bounce Ge(220) symmetric monochromator. Data were collected on the symmetric (0002), (0004), and (0006) and asymmetric (10–15), (12–31), and (10–12) reflections as reciprocal space mappings (RSMs) or just  scans. Doubledaxis rocking curves of the (10–15), (12–31), and (10–12) in ωscans and scans were recorded in skew diffraction geometry . The samples surface morphology was characterized by atomic force microscopy (AFM) in contact mode with a commercial VEECO CPII.
3. Results and Discussion
The surface morphology of the AlInN epilayers grown on GaN template layers is characterized by AFM. Figures 2(a) and 2(b) show the AFM image of the samples A and C. The rootmeansquare (RMS) roughness ( scan) varies between 0.3 nm (for sample A) and 6.9 nm (for sample C). Sample A has a smooth surface with low rms roughness compared to the other samples. The variation of the RMS roughness with indium content in an AlInN layer is shown in Table 1. Based on the observation from Table 1, the RMS roughness values of the AlInN layers did not show any systematic dependence on the indium content.

(a)
(b)
HRXRD measurements were performed for all of the samples to investigate the crystal phase of the AlInN epilayer on GaN template layer. Figure 3 shows the 2θωscan HRXRD pattern of (0002) peaks of the AlInN/GaN samples. The diffraction patterns exhibited the wurtzite AlInN epilayers with different indium concentration clearly observed at 35.91, 35.05, 34.99, 34.31, and 34.26° for samples A, B, C, D, and E, respectively. Also from Figure 3, the (0002) peaks of the wurtzite GaN template layers are seen at similar angle values. No peaks are identified except those corresponding to GaN template layers and InAlN epilayers. From Figure 3, no reflections other than those corresponding to GaN and InAlN can be identified, these results indicating that we have grown homogeneous material without phase separation and metal segregation.
In order to investigate the inplane alignment of an AlInN epilayer and GaN template layer, in which an inplane scan was also taken by rotating the sample around its surfacenormal direction, the scan patterns of the (10–15) plane of sample B are given in Figure 4. As can be seen in Figure 4, the diffraction peaks from the (10–15) plane of GaN and AlInN were observed at ~60° intervals, confirming the hexagonal structure of the AlInN epilayer and GaN template layer.
(a)
(b)
HRXRD provides highly precise measurement on the lattice parameters of a thin film. The Xray reciprocal space map (RSM) is a powerful tool for detailed structural characterization of imperfect crystalline layers [31, 32]. The RSM is based on twodimensional diffraction measurements in the scattering plane: in the perpendicular direction (i.e., 2θωscan) and in the parallel direction along the diffraction vector (i.e., ωscan). Correspondingly, a map taken from asymmetric reflection of the samples allows one to deduce both the inplane and the outofplane lattice parameters and thus to simultaneously determine the residual strain and stress as well as the exact alloy composition of the layers [31, 32]. The lattice parameter and can be determined by XRD directly from the reflections in the symmetric  scan by combining Bragg’s equation , where is the Miller index in notation, is the wavelength of the Xrays, and is the Bragg angle, with the expression for interplanar spacing in hexagonal structures given below [31, 32]:
In order to calculate values by using (1) at least two reflections measurements are needed (because of two unknowns ( and )). Generally, one or two highangle symmetric reflections are measured from the (0004), and/or (0006) planes, from which can be found directly [31]. On the other hand, the values can be calculated just with one or two highangle asymmetric reflections measurement (typically (10–15), (20–25), or (20–24) reflection). From highangle asymmetric reflections values can be determined by combining the value of found previously [31].
The lattice and thermal mismatch between the substrate and IIInitrides disallow growth directly on substrates (for example SiC, Al_{2}O_{3}, and Si as a substrate). Growth on high mismatched substrates can result in dislocations leading to domain walls and highly mosaic films. In order to improve the crystalline quality of the IIInitrides layers different type of buffer structures (e.g., LTAlN, LTGaN, HTGaN layer, etc.) needed to use between epilayers and substrates. The mosaic structures of the GaN growth on Si, SiC, and sapphire is strongly influenced by the growth conditions of the nucleation layer and is known to affect the electronic properties of thin films [8, 9]. In most cases, a GaN layer is used as a buffer layer [4, 11]. Between the groupIII nitride alloy film and the GaN buffer, a nearly perfect inplane orientation is established [8, 9]. In order to determine the strain and composition of the layer, commonly a peak from another IIInitride layer is used as the “substrate” [31]. If the material is assumed to be unstrained, then composition is the only factor affecting the lattice parameters and only lattice parameters need to be measured. For this case, Vegard’s law has been applied, which states that the lattice parameters of an alloy will vary linearly between the end members. For the unstrained and lattice parameter of AlInN (where is the mole fraction of InN), Vegard’s law is given by [8, 9, 31, 33]
If the strained lattice parameters and are known, the sample strain can be taken into account in estimates of the composition: where and are the measured lattice parameters (which take into account strain), and are the relaxed parameters predicted by Vegard’s law, and and are elastic constants linearly interpolated from the binary values. is the Poisson’s ratio for a hexagonal crystal system biaxially strained perpendicular to and is given by (4).
The linear relationship for the Poisson’s ratio as a firstorder approximation is given by
Substitution of , and into (3) obtained a cubic equation for given below
The coefficient (K, L, M, N) of (6) can be determined by a algebraic calculation. A more detailed , , and dependent coefficient K, L, M, N expression can be found in [33]. The solution of (6) gives the In mole fraction in the case of . There are three real solutions, but only one physically meaningful value of in the interval . By using calculated mole fraction , in (2), and (5), the relaxed lattice parameters of the AlInN alloy film and , as well as Poisson’s ratio , can be obtained. In order to perform the calculations, in addition to the measured lattice parameters, the relaxed lattice constants of the AlN (, ,) [31, 34] and the InN (, ,) [31, 34] and the elastic constant ( and GPa) for AlN and ( and GPa) InN [31, 34] are used as input parameters. The inplane and outofplane strain components can be defined as and , where and are the measured lattice parameters, while and are the relaxed parameters given by Vegard’s law [31, 33].
The RSM was performed for both symmetric (0002) and asymmetric (10–15) reflections of the GaN and AlInN layers. The  HRXRD RSM of the (0002) and (10–15) reflections of all of the AlInN/GaN (0001)/Al_{2}O_{3} samples are shown in Figures 5 and 6, respectively. From the RSM figure of the (0002) and (10–15) reflections, the pole position of the (0002) and (10–15) reflections of the GaN template layers and the AlInN layers can be seen clearly for samples A, B, and C, but for samples D and E, pole position of the AlInN layers could not be seen clearly, because of the close 2θ values of the GaN template layers and AlInN layers. The Indium content, lattice parameters, and strain values in the AlInN layers, in addition to the lattice parameters and the strain values of the GaN template layer, were calculated from the RSM around symmetric (0004) and asymmetric (10–15) reflection, whose values are given in Table 1. The and components for the AlInN epilayers were calculated and given in Table 1. The and values in the AlInN epilayers are one order bigger for samples D and E than the other samples. These results can be attributed to the lattice mismatch between GaN and AlInN with increasing In content in AlInN layer.
(a)
(b)
(c)
(d)
(e)
(a)
(b)
(c)
(d)
(e)
The GaN based layers usually grown on lattice mismatched substrate, such as sapphire, SiC, and Si, cause a high dislocation density. In our case, AlInN epilayers and GaN template were grown on sapphire substrate, which exhibit dislocation density. There are three main types of dislocations present in AlInN epilayers and GaN template layers [8–10, 23, 31]: the pure edge type dislocation with Burgers vector , the pure screw type dislocation with Burgers vector , and the mixed type dislocation with . The edge and screw type dislocation density in the epitaxial layers can be calculated with the equation given below [8–10, 23, 31]
In (7), the FWHM is measured by XRD rocking curves for (0002) and (10–12) reflections and is the Burgers vector length ( for GaN and burgers vector for AlInN used from Table 1). The total dislocation density of the AlInN epilayers and GaN template layers is the summation of the edge and screw type dislocation density.
The calculated edge and screw type dislocation densities of the GaN template layers and the AlInN epilayers are given in Table 2. As can be seen in Table 2, the screw type dislocation density in GaN template layers changes between (sample D) and cm^{−2} (sample A), but edge type dislocation densities are a little bit higher than screw type dislocation densities and change between (sample D) and cm^{−2} (sample C). The calculated dislocation density values for GaN layers are comparable with GaN, grown on similar buffer structure with MOCVD, reported in literature [8, 27]. In addition, the calculated screw and edge type dislocation densities in AlInN epilayers were given in Table 2. The calculated values of the screw type dislocation densities in AlInN epilayers were determined to range from (sample B) to cm^{−2} (sample D). On the other hand, the edge type dislocation densities in the AlInN epilayers change between (sample B) and cm^{−2} (sample E). Based on the observations in Table 2, in the AlInN epilayers, both screw and edge type dislocation densities are a little bit higher than in GaN template layers. Moreover, both for sample D and sample E ( and 0.48), the screw and edge type dislocation densities are higher than the other samples. These cases can be explained with an increasing mismatch in the results of increasing indium content in samples D and E.

AlInN epilayers having a large lattice mismatch with respect to the GaN template layers and substrate form a mosaic structure of slightly misoriented subgrains, which is characterized by the nucleation of slightly misoriented islands and the coalescence of these islands toward a smooth surface [8–10, 22–27]. The mosaic blocks can be defined as slightly misoriented with respect to each other. The vertical and lateral coherence lengths, heterogeneous strain, and degree of mosaicity expressed by the tilt and twist angles are important parameters in characterizing the quality of the epitaxial films [8, 9, 22–30]. The mosaic tilt and twist are defined as the outofplane rotation of the blocks perpendicular to the surface normal and the inplane rotation around the surface normal, respectively [8, 9, 22–30]. The average absolute values of the tilt and twist are directly related to the FWHM of the corresponding distributions of crystallographic orientations [22–27]. The lateral and vertical coherence length, tilt angle, and heterogeneous strain along the caxis parameters can be calculated from the WilliamsonHall (WH) plot, and the twist angle from approaches that were proposed by Srikant et al. [25] and Sun et al. [30] or from direct measurement [26, 27].
Each contribution to the broadening of particular XRD curves can be separated in a WH plot [21, 23, 31]. Specifically in tripleaxis diffractometer measurements, the broadening of the rocking curve (scan or angularscan) of the symmetric (0002), (0004), and (0006) reflections for the epitaxial layer is influenced only by the tilt angle and short coherence length parallel to the substrate surface [8, 9, 21, 23].
The is plotted against for each reflection and fitted by a straight line, where (FWHM)_{ω} is in the angular unit and taken as radians, is the Bragg’s reflection angle, and is the Xray wavelength. Then, the mean tilt angle () is calculated from the slope of the straight line, and the lateral coherence length () from the inverse of the yintersection of the fitted line with the ordinate.
Because of a small vertical correlation length and a heterogeneous strain along the axis causes a broadening of the Bragg reflections in the scan (or radialscan direction) of the symmetric reflections. These two parameters vertical coherence length () and vertical heterogeneous strain () can be easily derived from the WH plot. In the WH plot, is plotted against for each reflection and again fitted by a straight line [8, 9]. The values of the can be estimated directly from the slope (slope = ) of the line and the from the intersection () the vertical coherence length can be calculated from the intersection () point ().
The WH plots for symmetric plane ((0002), (0004), (0006)) reflections of the AlInN epilayers were done for the tripleaxis  and scan. Figure 7 shows the corresponding WH plots of the AlInN epilayers for the tripleaxis (a) scan and (b) scan. The straight lines are linear fits to the experimental data. The expected linear behavior of the graphs is experimentally well confirmed, which gives rather accurate tilt angle values.
(a)
(b)
The and of the AlInN epilayers are shown in Table 3. The values of the samples change between the 0.080 and 0.238 degree. As can be seen in table, the of the samples A, B, and C are similar to each other and rather small. However, with increasing In content, the mean tilt angles increased approx. twofold and measured as 0.221 and 0.238 degree for samples D and E, respectively. Based on the observation of the measured values, it can be concluded that the increased indium content ratio in the AlInN epilayers affects the mean tilt mosaic of the mosaic blocks of the AlInN epilayers.

The of the AlInN epilayers were determined to range from 559.1 to 2000.1 nm. As can be seen in Table 3, the maximum values were observed for sample D and the minimum values obtained for sample C. The measured values for AlInN epilayers are shown in Table 3. The values for AlInN epilayers range from 28.3 (sample B) to 294.1 nm (sample E). The values that were calculated for the GaN template layers and AlInN epilayers for all samples are shown in Table 3. The maximum values in the AlInN epilayers were obtained for sample E.
Generally, the mean twist angle () between the subgrains of AlInN and GaN epilayers can be determined from the FWHM of scan or scan XRD curves [8, 9, 22–26]. The mean twist angle can be extrapolated from a fit to the measured doubleaxis scans data for different reflections in a skew symmetric diffraction. Several extrapolation and direct measurements methods have been reported in the literature for a mean twist angle calculation [25, 26, 28, 30]. Srikant et al. [25] and Sun et al. [30] proposed a geometrical model that considers the simultaneous presence of tilt and twist to fit the data from the measurement of scans in skew geometry from reflections with increasing lattice plane inclination (χ). Actually, these authors obtained the twist angle by the complicated calculation and fitting method. Metzger et al. [23] just used the FWHM of scan for (10–15) reflection to measure the twist angle. On the other hand, some authors proposed a simple empirical approach to obtain the mean twist angle directly without falling into complicated computation and fitting procedure [26, 27]. In the other measurement method is the grazing incidence inplane Xray diffraction (GIIXD) technique, but in this technique a high intensity Xray source such as a synchrotron and/or special Xray optics is necessary [35, 36].
The FWHM of the rocking curve of an imperfect film is composed of several contributions, such as the mean tilt, twist, the average size of the subgrains, and the inhomogeneous strain distributions. Although the broadening, due to a limited domain size and inhomogeneous strain, can be significant in highly imperfect films, their effects have been eliminated by using a slit of 0.6 mm that is placed in front of the detector in doubleaxis scans. Indeed, their contribution to the overall broadening was found to be of minor influence in this measurement case. In addition, the (0002) reflection and reflections with either or nonzero orientation of our samples with tripleaxis scans exhibit a small FWHM. The last important point is that the intrinsic width of the reflection for the crystal and the apparatus broadening for all the experimental reflections are negligible because these effects amount to only a few arcsec. For this reason, we can only measure the broadening that was caused by the twist only by using reflections in skew geometry [8–10, 27].
Doubledaxis rocking curves of the scans and scans in different were recorded in skew diffraction geometry . In Figure 8, the FWHMs values changes of the and scans with an increasing inclination angle () for the sample A were given. The extended FWHMs of and scans are obtained by using the fit of PseudoVoigt function to the rocking curves. It can be seen in this figure that the FWHMs of scans increase with the increment of , while the FWHM of scan decreases with the increment of angle. Moreover, they become closer when the (12–31) reflection yields at 78.6° in as seen in Figure 8. In fact, the angle reaches 90° when the reflection plane is perpendicular to the surface of the sample. These results showed that the rockingcurve widths of or scans for this higher angle are close to the twist angles. In every respect, the FWHMs of scans are larger than those of scans with the change of the inclination angle . Therefore, the mean twist angles must be the average value of the FWHMs of and scans at = 78.6°.
The measured mean twist angles of the AlInN epilayers are shown in Table 3. The measured mean twist angles of the AlInN epilayers change between 0.100° and 0.248°. It can be concluded that the mean twist angles in the AlInN epilayers are close to each other for all the samples. The minimum mean twist angle value was obtained as 0.100° for sample D, while the maximum mean twist angle was obtained as 0.248° for sample C. Based on this observation, it can be argued that the mean twist angle of the AlInN epilayers grown on a GaN template was not strongly affected by the indium content () of the epilayers.
4. Conclusions
In the present study, epitaxial layers, with indium content of 0.04, 0.18, 0.20, 0.47, and 0.48, were grown on GaN template/sapphire structure by MOCVD. The mosaic structures parameters (such as lateral and vertical coherence lengths, tilt and twist angle, and heterogeneous strain) and dislocation densities (edge and screw type dislocations) of the AlInN epilayers and GaN template layers were investigated by using HRXRD measurements. Based on the HRXRD measurements results, we observed that the mosaic structures parameters, lateral and vertical coherence lengths, tilt and twist angle, and heterogeneous strain of the AlInN epilayers were not strongly affected by indium content in epilayers. The screw type dislocation density in GaN template layers changes between (sample D) and cm^{−2} (sample A), but edge type dislocation densities are a little bit higher than screw type dislocation densities and change between (sample D) and cm^{−2} (sample C). The calculated values of the screw type dislocation densities in AlInN epilayers were determined to range from (sample B) to (sample D). On the other hand, the edge type dislocation densities in the AlInN epilayers are changes between (sample B) and cm^{−2} (sample E).
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
Acknowledgments
This work is supported by the European Union under the projects EUMETAMORPHOSE, EUPHOREMOST, EUPHOME, and EUECONAM, and TUBITAK under Project nos. 105E066, 105A005, 106E198, and 106A017. One of the authors (Ekmel Ozbay) also acknowledges partial support from the Turkish Academy of Sciences.
References
 H. Morkoç, Nitride Semiconductors and Devices, Springer, Heidelberg, Germany, 1999.
 S. Nakamura and G. Fasol, The Blue Laser Diode GaN based Light Emitters and Lasers, Springer, Heidelberg, Germany, 1997.
 F. A. Ponce and D. P. Bour, “Nitridebased semiconductors for blue and green lightemitting devices,” Nature, vol. 386, pp. 351–359, 1997. View at: Publisher Site  Google Scholar
 O. Ambacher, “Growth and applications of group IIInitrides,” Journal of Physics D: Applied Physics, vol. 31, p. 2653, 1998. View at: Publisher Site  Google Scholar
 E. Arslan, S. Turan, S. Gökden, A. Teke, and E. Özbay, “CurrentTransport Mechanisms in the AlInN/AlN/GaN singlechannel and AlInN/AlN/GaN/AlN/GaN doublechannel heterostructures,” Thin Solid Films, vol. 548, pp. 411–418, 2013. View at: Publisher Site  Google Scholar
 B. S. Eller, J. L. Yang, and R. J. Nemanich, “Electronic surface and dielectric interface states on GaN and AlGaN,” Journal of Vacuum Science & Technology A, vol. 31, no. 5, Article ID 050807, 2013. View at: Publisher Site  Google Scholar
 R. S. Pengelly, S. M. Wood, J. W. Milligan, S. T. Sheppard, and W. L. Pribble, “A review of GaN on SiC high electronmobility power transistors and MMICs,” IEEE Transactions on Microwave Theory and Techniques, vol. 60, no. 6, pp. 1764–1783, 2012. View at: Publisher Site  Google Scholar
 E. Arslan, M. K. Ozturk, H. Çakmak, P. Demirel, S. Özçelik, and E. Ozbay, “Evolution of the mosaic structure in InGaN layer grown on a thick GaN template and sapphire substrate,” Journal of Materials Science: Materials in Electronics, vol. 24, no. 11, pp. 4471–4481, 2013. View at: Publisher Site  Google Scholar
 E. Arslan, M. K. Ozturk, A. Teke, S. Ozcelik, and E. Ozbay, “Buffer optimization for crackfree GaN epitaxial layers grown on Si(1 1 1) substrate by MOCVD,” Journal of Physics D: Applied Physics, vol. 41, no. 15, Article ID 155317, 2008. View at: Publisher Site  Google Scholar
 J. S. Speck and S. J. Rosner, “The role of threading dislocations in the physical properties of GaN and its alloys,” Physica B, vol. 24, no. 1–3, pp. 273–274, 1999. View at: Google Scholar
 L. Liu and J. H. Edgar, “Substrates for gallium nitride epitaxy,” Materials Science and Engineering R, vol. 37, no. 3, pp. 61–127, 2002. View at: Google Scholar
 J. Xie, X. Ni, M. Wu, J. H. Leach, U. Özgür, and H. Morkoç, “High electron mobility in nearly latticematched AlInN/AlN/GaN heterostructure field effect transistors,” Applied Physics Letters, vol. 91, no. 13, Article ID 132116, 2007. View at: Google Scholar
 H. Behmenburg, L. Rahimzadeh Khoshroo, M. Eickelkamp et al., “Influence of barrier thickness on AlInN/AlN/GaN heterostructures and device properties,” Physica Status Solidi C, vol. 6, supplement 2, pp. S1041–S1044, 2009. View at: Publisher Site  Google Scholar
 G. Liu, J. Zhang, X.H. Li et al., “Metalorganic vapor phase epitaxy and characterizations of nearlylatticematched AlInN alloys on GaN/sapphire templates and freestanding GaN substrates,” Journal of Crystal Growth, vol. 340, no. 1, pp. 66–73, 2012. View at: Publisher Site  Google Scholar
 L. F. Jiang, W. Z. Shen, and Q. X. Guo, “Temperature dependence of the optical properties of AlInN,” Journal of Applied Physics, vol. 106, Article ID 013515, 2009. View at: Publisher Site  Google Scholar
 T. Aschenbrenner, H. Dartsch, C. Kruse et al., “Optical and structural characterization of AlInN layers for optoelectronic applications,” Journal of Applied Physics, vol. 108, Article ID 063533, 2010. View at: Publisher Site  Google Scholar
 M. M. Satter, H.J. Kim, Z. Lochner et al., “Design and analysis of 250nm AlInN laser diodes on AlN substrates using tapered electron blocking layers,” IEEE Journal of Quantum Electronics, vol. 48, no. 5, pp. 703–711, 2012. View at: Publisher Site  Google Scholar
 A. Minj, D. Cavalcoli, and A. Cavallini, “Indium segregation in AlInN/AlN/GaN heterostructures,” Applied Physics Letters, vol. 97, Article ID 132114, 2010. View at: Google Scholar
 J. J. Zhu, Y. M. Fan, H. Zhang et al., “Contribution of GaN template to the unexpected Ga atoms incorporated into AlInN epilayers grown under an indiumveryrich condition by metalorganic chemical vapor deposition (MOCVD),” Journal of Crystal Growth, vol. 348, no. 1, pp. 25–30, 2012. View at: Publisher Site  Google Scholar
 C. Hums, J. Bläsing, A. Dadgar et al., “Metalorganic vapor phase epitaxy and properties of AlInN in the whole compositional range,” Applied Physics Letters, vol. 90, no. 2, Article ID 022105, 2007. View at: Publisher Site  Google Scholar
 G. K. Williamson and W. H. Hall, “Xray line broadening from filed aluminium and wolfram,” Acta Metallurgica, vol. 1, no. 1, pp. 22–31, 1953. View at: Publisher Site  Google Scholar
 V. Holy, J. Kubena, E. Abramof, K. Lischka, A. Pesek, and E. Koppensteiner, “X‐ray double and triple crystal diffractometry of mosaic structure in heteroepitaxial layers,” Journal of Applied Physics, vol. 74, article 1736, 1993. View at: Publisher Site  Google Scholar
 T. Metzger, R. Höppler, E. Born et al., “Defect structure of epitaxial GaN films determined by transmission electron microscopy and tripleaxis Xray diffractometry,” Philosophical Magazine A, vol. 77, p. 1013, 1998. View at: Publisher Site  Google Scholar
 M. E. Vickers, M. J. Kappers, R. Datta et al., “Inplane imperfections in GaN studied by xray diffraction,” Journal of Physics D: Applied Physics, vol. 38, no. A99, 2005. View at: Publisher Site  Google Scholar
 V. Srikant, J. S. Speck, and D. R. Clarke, “Mosaic structure in epitaxial thin films having large lattice mismatch,” Journal of Applied Physics, vol. 82, p. 4286, 1997. View at: Publisher Site  Google Scholar
 H. Heinke, V. Kirchner, S. Einfeldt, and D. Hommel, “Xray diffraction analysis of the defect structure in epitaxial GaN,” Applied Physics Letters, vol. 77, p. 2145, 2000. View at: Publisher Site  Google Scholar
 X. H. Zheng, H. Chen, Z. B. Yan et al., “Determination of twist angle of inplane mosaic spread of GaN films by highresolution Xray diffraction,” Journal of Crystal Growth, vol. 255, pp. 63–67, 2003. View at: Publisher Site  Google Scholar
 H. Li, Y. Luo, L. Wang et al., “Determination of the twist angle of GaN film by high resolution Xray diffraction,” Applied Physics Express, vol. 1, Article ID 045004, 2008. View at: Publisher Site  Google Scholar
 R. Chierchia, T. Böttcher, H. Heinke, S. Einfeldt, S. Figge, and D. Hommel, “Microstructure of heteroepitaxial GaN revealed by xray diffraction,” Journal of Applied Physics, vol. 93, no. 11, pp. 8918–8925, 2003. View at: Publisher Site  Google Scholar
 Y. J. Sun, O. Brandt, T. Y. Liu et al., “Determination of the azimuthal orientational spread of GaN films by xray diffraction,” Applied Physics Letters, vol. 81, p. 4928, 2002. View at: Publisher Site  Google Scholar
 M. A. Moram and M. E. Vickers, “Xray diffraction of IIInitrides,” Reports on Progress in Physics, vol. 72, Article ID 036502, 2009. View at: Google Scholar
 P. E. Fewster, “Reciprocal space mapping,” Critical Reviews in Solid State and Materials Sciences, vol. 22, pp. 69–110, 1997. View at: Publisher Site  Google Scholar
 M. Schuster, P. O. Gervais, B. Jobst et al., “Determination of the chemical composition of distorted InGaN/GaN heterostructures from xray diffraction data,” Journal of Physics D: Applied Physics, vol. 32, no. 10, p. A56, 1999. View at: Publisher Site  Google Scholar
 A. F. Wright, “Elastic properties of zincblende and wurtzite AlN, GaN, and InN,” Journal of Applied Physics, vol. 82, p. 2833, 1997. View at: Publisher Site  Google Scholar
 T. A. Lafford, B. K. Tanner, and P. J. Parbrook, “Direct measurement of twist mosaic in GaN epitaxial films as a function of growth temperature,” Journal of Physics D: Applied Physics, vol. 36, no. 11, article A245, 2003. View at: Publisher Site  Google Scholar
 M. S. Goorsky and B. K. Tanner, “Grazing incidence inplane diffraction measurement of inplane mosaic with microfocus xray tubes,” Crystal Research and Technology, vol. 37, pp. 645–653, 2002. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2014 Engin Arslan et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.